Impact and Chemical Tests on Natural Fiber
Reinforced Epoxy Composite Material
K M D Mazharuddin1
, B Madhusudhan Reddy2
, H. Raghavendra Rao3
P.G. Student, Dept. of Mechanical Engineering, GPR Engineering College, Kurnool, A.P, India1
Assistant Professor, Dept. of Mechanical Engineering, GPR Engineering College, Kurnool, A.P., India2
Associate Professor, Dept. of Mechanical Engineering, GPR Engineering College, Kurnool, A.P., India3
ABSTRACT: Natural fibers are the other alternative in which the research is being carried out to overcome the problem of using metals due to its distinct characteristics like low cost, less weight, biodegradability etc. In this paper an attempt is made to prepare two different composite materials using Rose Madder (Rubia Cordifolia) and Burmese Silk Orchid (Bauhinia Racemosa) as reinforcement and Epoxy as the matrix material respectively. Composites were prepared by increasing the weight of fibers like 5,10,15,20 grams for reinforcement respectively by Hand Layup technique. Impact testing of the material was done by cutting the material into ASTM standards on an IZOD Impact Tester. Chemical tests were conducted for the respective composite materials by cutting some specimen from the material and immersing it in the chemicals like Sodium Hydroxide, Benzene, Toluene, Ammonium Hydroxide etc. It was found that as the weight of fiber increases there is improvement in the impact properties of the composite material and also its chemical properties towards various chemicals
KEYWORDS: composite, Natural Fibers, epoxy, hand layup, impact, chemical
Fig.1 types of reinforcements
Fibers are of two types, namely natural fibers and synthetic fibers. Natural fibers such as bamboo, sisal, jute etc are used as reinforcement and either thermoset or a thermoplastic are used as matrix. Synthetic fibers are polysters, aramide, nylon etc. The fibers may be continuous (long) or discontinuous (short).
The matrix must have a mechanical strength commensurate with that of the reinforcement i.e. both should be compatible. Thus, if a high strength fibre is used as the reinforcement, there is no point using a low strength matrix, which will not transmit stresses efficiently to the reinforcement. The matrix must stand up to the service conditions, viz., temperature, humidity, exposure to ultra-violet environment, exposure to chemical atmosphere, abrasion by dust particles, etc. It should not be toxic and should have a high flash point.
Rose Madder (Rubia Cordifolia) and Burmese Silk Orchid (Bauhinia Racemosa) fibers were peeled off from the barks collected from their respective trees which are present in Nallamalla forest at Bailrooty area in Andhra Pradesh. Fibers are cut to a length equal to the length of the mould. Epoxy mixed with hardener was used as matrix material. Epoxy and hardener were mixed at a ratio of 20:1 respectively. Glass mould with the dimensions 200mm x 200mm x 3mm (length x width x thickness) was used for the preparation of the composite. Other ingredients which were helpful in preparing the composite are releasing agent, OHP paper and a roller.
The material is cut into ten specimens with dimensions 10mm x 5mm x 3mm for chemical test as per ASTMD 543-87 specifications. The preweighted specimens were immersed in ten different chemicals for 24 hours in a test tube and then were removed, rinsed with distilled water and dried by pressing them on both sides with a filter paper at room temperature. The specimens were reweighted and the % weight gain/loss was recorded with the formula below.
𝑊 =w2− w1
Where W - Gain/loss weight of final specimen.
w1 - weight of specimen before immersing in chemical. w2 - weight of specimen after immersing in chemical.
The material is cut into specimens with dimensions 120mm x 13mm x 3mm and a notch was made at the centre of the specimen at 45 degrees angle for impact testing as per ASTMD 256-88 specifications. The impact strength of the specimen is determined using IZOD impact tester.
The IZOD Impact tester consists of a pendulum of known mass and length that is dropped from a known height to impact a notched specimen of the material. For this test a notched specimen is fixed between supports. The machine has the following specifications. The image of machine is shown in Fig.2.
Display : Digital Indicating Unit. Scale range : 2, 4, 7.5,15,25 Joules.
Hammers : Two.
Power supply : 230V AC, 50Hz, Single Phase.
IV.RESULTS AND DISCUSSION
Chemicals used for the tests are Nitric acid, Hydrochloric acid, Acetic acid, Sodium Hydroxide, Sodium Carbonate, Ammonium Hydroxide, Benzene, Toluene, Carbon Tetrachloride and Distilled water. The test is performed carefully so that our hands are not exposed directly to the chemicals. Table I and Table II show the chemical test values of the specimens of Rose Madder and Burmese Silk Orchid fiber reinforced epoxy matrix composites respectively. Weight of specimen before immersing in chemical (w1) and weight of specimen after immersing for 24 hours (w2) are noted and the gain/loss weight of the specimen (W) is calculated.
CHEMICAL TEST VALUES OF ROSE MADDER
Chemicals W1 W2 𝐖 =
40% nitric acid 0.32 0.29 -0.09
10% Hydrochloric acid 0.31 0.32 +0.03
8% Acetic acid 0.29 0.32 +0.103 10% sodium hydroxide 0.24 0.30 +0.25
20% sodium carbonate 0.26 0.31 +0.19
10% Ammonium Hydroxide 0.31 0.39 +0.25 Benzene 0.27 0.36 +0.33 Toluene 0.23 0.22 -0.04 Carbon tetrachloride 0.27 0.32 +0.18 Distilled Water 0.20 0.22 +0.1
CHEMICAL TEST VALUES OF BURMESE SILK ORCHID
Chemicals W1 W2 𝐖 =
40% nitric acid 0.21 0.24 +0.142
10% Hydrochloric acid 0.15 0.20 +0.33
8% Acetic acid 0.20 0.27 +0.35
10% sodium hydroxide 0.20 0.25 +0.25 20% sodium carbonate 0.17 0.21 +0.23 10% Ammonium Hydroxide 0.24 0.27 +0.12
Benzene 0.29 0.32 +0.10
Toluene 0.26 0.29 +0.11
The weight of fiber is taken as 5,10,15,20 grams respectively. First the pure epoxy is tested and then the fiber reinforced composites are tested with different fiber weights.
The IZOD unit calculations were as shown below:
1. Joule/Meter = 𝑆𝑐𝑎𝑙𝑒 𝑅𝑒𝑎𝑑𝑖𝑛𝑔 𝐽𝑜𝑢𝑙𝑒 𝐼𝑛𝑠𝑡𝑟𝑢𝑚𝑒𝑛𝑡
𝑆𝑎𝑚𝑝𝑙𝑒 𝑇𝑖𝑐𝑘𝑛𝑒𝑠𝑠 𝑖𝑛 𝑀𝑒𝑡𝑒𝑟𝑠
2. Kg.cm/cm= 𝑆𝑐𝑎𝑙𝑒 𝑅𝑒𝑎𝑑𝑖𝑛𝑔 𝐽𝑜𝑢𝑙𝑒 𝐼𝑛𝑠𝑡𝑟𝑢𝑚𝑒𝑛𝑡
𝑇𝑖𝑐𝑘𝑛𝑒𝑠𝑠 𝑜𝑓 𝑠𝑎𝑚𝑝𝑙𝑒 𝑖𝑛 𝑐𝑚 𝑋 10.1972
Fig.3 and Fig.4 shows the Impact specimens of Burmese Silk Orchid fiber and Rose Madder fiber composites respectively
Fig.3 Burmese Silk Orchid fiber composite impact specimen Fig.4 Rose Madder composite impact specimen
Table III and Table IV show the Impact testing values of Rose Madder and Burmese Silk Orchid fibers reinforced epoxy matrix composites respectively.
IMPACT TESTING VALUES OF ROSE MADDER
Weights of Fibers in
Kg.cm/cm (ASTM) 0 grams
(pure epoxy) 0.11 36.6 3.73
5 grams 0.97 323.33 32.97
10 grams 1.21 403.33 41.12
15 grams 1.43 476.66 48.6
IMPACT TESTING VALUES OF BURMESE SILK ORCHID
Weights of Fibers in
(pure epoxy) 0.11 36.6 3.73
5 grams 0.80 266.66 27.19
10 grams 1.12 373.33 38.06
15 grams 1.37 456.66 46.56
20 grams 1.63 543.33 55.40
From the results of both the tests we can conclude that both Rose Madder and Burmese Silk Orchid are almost have less weight changes towards different chemicals so we can use these both fiber reinforced composites in areas which are prone to acidic activity and can be used in various other applications like inner coverings in water tanks etc. The impact strengths of both the fibers show that as the fiber weight increases within a composite those composites have better impact strengths. Rose Madder fiber composite has higher impact strength than Burmese Silk Orchid fiber composite. From the broken pieces while performing impact testing show that breakage is caused due to small voids between the fibers and matrix material due to which there will be lesser adhesion between the fiber surface and the matrix material. So care should be taken to avoid formation of cavities within the composite while performing hand layup technique
 Vemu Vara Prasad, Mattam Lava Kumar, Chemical Resistance and Tensile Properties of Bamboo and Glass Fibers Reinforced Epoxy Hybrid Composites International Journal of Materials and Biomaterials Applications 2011; 1 (1):pp.17-20
 Raghavendra Yadav Eagala, Allaka Gopichand, Gujjala Raghavendra, Sardar Ali S, Abrasive Wear Behaviour of Bamboo-Glass Fiber Reinforced Epoxy Composites using Taguchi Approach International Journal of Advances in Engineering & Technology, Nov. 2012 Vol. 5, Issue 1, pp.399-405
 H. Raghavendra Rao, M. Ashok Kumar, G. Ramachandra Reddy, Hybrid composites: Effect of fibers on mechanical properties International Journal of Macromolecular Science 2011; 1(1): pp.9-14
 Md. Rashnal Hossain, Md. Aminul Islam, Aart Van Vuurea, Ignaas Verpoest, Tensile behavior of environment friendly jute epoxy laminated composite www.sciencedirect.com Procedia Engineering 56 ( 2013 ) pp.782 – 788
 C.S. Verma, V.M. Chariar, R. Purohit, Tensile Strength Analysis of bamboo and Layered Laminate Bamboo composites ISSN: 2248-9622 www.ijera.com Vol. 2, Issue 2,Mar-Apr 2012, pp.1253-1264
 R.Sakthivel, D.Rajendran, Experimental Investigation and Analysis a Mechanical Properties of Hybrid Polymer Composite Plates International Journal of Engineering Trends and Technology (IJETT) – Volume 9 Number 8 - Mar 2014 pp.407-414
 V.P. Arthanarieswaran, A. Kumaravel, M. Kathirselvam, Evaluation of mechanical properties of banana and sisal fiber reinforced epoxy composites: Influence of glass fiber hybridization www.sciencedirect.com Materials and Design 64 (2014) pp.194–202
 V.S. Srinivasan, S. Rajendra Boopathy, D. Sangeetha, B. Vijaya Ramnath, Evaluation of mechanical and thermal properties of banana–flax based natural fibre composite www.sciencedirect.com Materials and Design 60 (2014) pp.620–627
 U. Sule, T. Isa, A. O. Ameh, O. A. Ajayi, O. Omorogbe, Studies on the Properties of Short Okra/Glass Fibers Reinforcedepoxy Hybrid Composites The International Journal Of Science & Technoledge Vol 2 Issue 7 July, 2014 pp.260-26